## Abstract

Topological quantum materials represent a new class of matter with both exotic physical phenomena and novel application potentials. Many Heusler compounds, which exhibit rich emergent properties such as unusual magnetism, superconductivity and heavy fermion behaviour, have been predicted to host non-trivial topological electronic structures. The coexistence of topological order and other unusual properties makes Heusler materials ideal platform to search for new topological quantum phases (such as quantum anomalous Hall insulator and topological superconductor). By carrying out angle-resolved photoemission spectroscopy and *ab initio* calculations on rare-earth half-Heusler compounds LnPtBi (Ln=Lu, Y), we directly observe the unusual topological surface states on these materials, establishing them as first members with non-trivial topological electronic structure in this class of materials. Moreover, as LnPtBi compounds are non-centrosymmetric superconductors, our discovery further highlights them as promising candidates of topological superconductors.

## Introduction

Topological quantum materials, a new class of matter with non-trivial topological electronic structures, has become one of the most intensively studied fields in physics and material science due to their rich scientific significance and broad application potentials^{1,2}. With the worldwide effort, there have been numerous materials predicted and experimentally confirmed as topologically non-trivial matter (including topological insulators^{3,4}, topological crystalline insulators^{5,6} and three-dimensional (3D) topological Dirac and Weyl semimetals^{7,8,9,10,11}). However, there is a big family of materials—the Heusler compounds—although being theoretically predicted to be topologically non-trivial back in 2010 (refs 12, 13, 14), the non-trivial topological nature has never been experimentally confirmed up to date.

The ternary semiconducting Heusler compounds, with their great diversity (∼500 members, >200 are semiconductors) give us the opportunity to search for optimized parameters (for example, spin–orbit coupling (SOC) strength, gap size and so on) across different compounds—which is critical not only for realizing the topological order and investigating the topological phase transitions^{12}, but also for designing realistic applications. In addition, among the wealth of Heusler compounds, many (especially those containing rare-earth elements with strongly correlated *f* electrons) exhibit rich interesting ground state properties, such as magnetism^{15,16}, superconductivity^{17,18,19} or heavy fermion behaviour^{20}. The interplay between these properties and the topological order makes Heusler compounds ideal platforms for the realization of novel topological effects (for example, exotic particles including image monopole effect and axions and so on), new topological phases (for example, topological superconductors^{21,22}) and broad applications (see ref. 23 for a review).

Rare-earth half-Heusler compounds LnPtBi (Ln=Y, La and Lu) represent a model system recently proposed that can possess topological orders with non-trivial topological surface states (TSSs) and large band inversion^{12,24}. Moreover, due to the lack of the inversion symmetry in their crystal structure, non-centrosymmetric superconducting LnPtBi compounds (Tc=0.7^{17}, 0.9^{18} and 1.0 K^{19} for Ln=Y, La and Lu, respectively) may also host unconventional cooper pairs with mixed parity, making them promising candidates for the investigation of topological superconductivity and the search for Majorana fermions^{25}.

However, despite the great interests and intensive research efforts in both theoretical^{12,13,26} and experimental^{27,28,29} investigations, the topological nature on LnPtBi remains elusive. A previous angle-resolved photoemission spectroscopy (ARPES) study has reported metallic surface states^{27} with apparently different dispersion shapes and Fermi surface (FS) crossing numbers from the predicted TSSs in LnPtBi compounds^{12,13}, making the topological nature of LnPtBi controversial.

In this work, by carefully performing comprehensive ARPES measurements and *ab initio* calculations, we resolve this unsettled question. We observe the non-trivial TSSs with linear dispersions in half-Heusler compounds LuPtBi and YPtBi (on the Bi-and Y-terminated (111) surface, respectively); and remarkably, in contrast to many topological insulators that have TSSs inside their bulk gap^{1,3,30}, the TSSs in LnPtBi show their unusual robustness by lying well below the Fermi energy (*E*_{F}) and strongly overlapping with the bulk valence bands (similar to those in HgTe^{31,32,33}). In addition to the TSSs, we also observe numerous metallic surface states crossing the *E*_{F} with large Rashba splitting, which not only makes them promising compounds for spintronic application, but also provides the possibility to mediate topologically non-trivial superconductivity in the superconducting phase of these compounds.

## Results

## Basic physical properties of LnPtBi

A crystallographic unit cell of LnPtBi is shown in Fig. 1a, which comprises of a zinc-blend unit cell from Bi and Pt atoms and rocksalt unit cell from Bi and Ln. For ARPES measurements, the LnPtBi single crystals were cleaved *in situ* in the ultra-high vacuum measurement chamber, resulting in either (111) or (001) surfaces. The unit cell along the (111) cleavage surface is illustrated in Fig. 1b and the corresponding hexagonal surface Brillouin zone (BZ) is shown in Fig. 1d, which could be viewed as the projection of the bulk BZ (Fig. 1c) of LnPtBi along the [111] direction (Fig. 1d).

The unit cell along the [111] direction consists of alternating Ln, Pt and Bi layers (Fig. 1b). As there are fewer chemical bonds to break between Ln and Bi layer (two comparing to three between Ln and Pt or Pt and Bi layers) and the Ln–Bi layer distance is twice as large as the Ln–Pt or Pt–Bi layer spacing (see Fig. 1b), it is more energetically favourable to cleave the material between Ln and Bi layers. In the discussion of the main text, we will focus on the electronic structure of Bi-terminated (111) surface LuPtBi and Y-terminated (111) surface of YPtBi. ARPES results (as well as *ab initio* calculations) along (001) cleavage surfaces of LuPtBi and YPtBi are presented in Supplementary Information.

The core level photoemission spectra of LuPtBi is shown in Fig. 1e, from which the characteristic Bi *5d* and Lu *4f* doublets are clearly observed. The large spectral weight of Bi peaks over the Lu peaks in the (111) surface clearly indicates its Bi termination. The broad area FS mapping covering multiple BZs in Fig. 1f also illustrates the hexagonal symmetry (with the correct lattice parameters) resulting from the (111) cleaved surface.

## General electronic structure of LuPtBi (111) surface

In Fig. 2, detailed electronic structures of LuPtBi within a surface BZ are illustrated. From the FS maps (Fig. 2a–c) and 3D spectral intensity plots (Fig. 2d,e) around both the point and BZ boundary ( and points), there are clearly multiple bands crossing *E*_{F}, forming a twin hexagonal hole pockets at and complex electron pockets at and , both of which show clear Rashba splitting. Around , there is another pair of double Λ shape hole bands just below *E*_{F}. These features broadly agree with the previous ARPES report^{27} (also see Supplementary Figs 1 and 2 and Supplementary Note 1 for the detailed discussions on the features near ). However, in this work, with the high instrument resolution and data statistics we successfully observed a critical additional X shape band dispersing between 0.4 and 0.8 eV with the band crossing point (that is, Dirac point) at *E*_{b}∼0.5 eV at the point—which is the long-sought-after TSSs, as we will discuss in details below.

## Surface states on LuPtBi (111) surface

To help understand the origin of these electronic states, we carried out band structure calculations of Bi-terminated LuPtBi (111) surface with two different methods (Fig. 3a,b, see the ‘Methods’ section for more details), and both agree well with the measurement and clearly reproduce the X shape TSS observed in our measurements (Fig. 3c–f). In Fig. 3a, we first employed a slab model for the *ab initio* calculations (method one). This method, which takes into account the charge density redistribution due to surface potential modification by *ab initio* calculations, can describe all surface states including TSSs and those from the trivial dangling bonds. To further identify the TSS, we carried out another method (Fig. 3b) by calculating the k-resolved local density of states of a semi-infinite surface using the recursive Green's function (method two)^{34} constructed from Wannier function-based tight-binding parameters extracted from the bulk material^{35}. Such method could reveal TSSs clearly and avoid the trivial surface states by removing the dangling bond orbitals in the Hamiltonian (as can be clearly seen in Fig. 3b).

The combination of the two methods thus allows us to unambiguously identify the TSSs from other trivial dangling bond states (further experimental evidence of the non-trivial nature of the TSSs can be found in Supplementary Fig. 3 and Supplementary Note 2). As shown in Fig. 3a, all sharp dispersions (three Kramers pairs and one X shape state, labelled as SS1–SS3 and TSS respectively) are of surface origin and agree excellently with the observed band structures (Fig. 3c–f). Moreover, the three Kramers pairs (SS1, SS2 and SS3) are all absent in the result from method two (Fig. 3b) while the X shape band remains, illustrating their topologically trivial origin (that is, being trivial surface states due to dangling bonds), as opposite to the TSS shown in Fig. 3b.

The surface origin of both the TSS and SS1–SS3 in Fig. 3 can also be experimentally verified by performing the photon energy dependence photoemission measurement^{30}, as presented in Fig. 4 (also in Supplementary Fig. 4 and Supplementary Note 3 along the other high symmetry direction). In Fig. 4a, dispersions along –– directions measured using a wide range of photon energies (50–75 eV) were plotted, the dispersions of TSS and SS1–SS3 under all photon energies are identical (though the relative intensity can vary with photon energy due to the photoemission matrix element effect^{30}). To further visualize the dispersion of these bands along *k*_{z}, we extract the momentum distribution curves (MDCs) at *E*_{F} (cutting through SS1 and SS2) and 0.65 eV below *E*_{F} (cutting through TSS, SS2 and SS3) and plot them as the function of photon energy (see Fig. 4b,c). Evidently, the peaks from TSS and SS1–SS3 bands show no *k*_{z} dispersion as they all form straight vertical lines. Thus, the surface nature of these bands (TSS and SS1–SS3) are clearly established. By fitting the Dirac type X shape linear dispersion (Fig. 4d), we can extract the band velocity at the Dirac point as 2.37 eV Å (3.59 × 10^{5} m s^{−1}) and 3.13 eV Å (4.74 × 10^{5} m s^{−1}) along the – and – direction, respectively.

## Surface states on YPtBi (111) and LnPtBi (001) surface

Similarly, for the other compound YPtBi, our calculation and measurements also agree well and both clearly show the TSS (Fig. 4e–g, also see Supplementary Fig. 5 and Supplementary Note 4 for the calculation). More measurements, as well as calculations on different cleaved surfaces (001) and different termination layers (Bi or Ln terminations), are presented in Supplementary Figs 6 and 7 and Supplementary Note 5, all showing excellent agreements. Interestingly, in both compounds, the observed TSS coexist and overlap in energy with the bulk valence band (appear as broad dispersing background intensity in Figs 3 and 4), demonstrating its unusual robustness.

## Circular dichroism (CD)-ARPES of LuPtBi surface states

CD-ARPES measurement on the Bi-terminated (111) surface of LuPtBi has also been carried out (see Fig. 5). As one can see from the cut along the – direction, the photoemission spectra intensity under circularly polarized right (CR) or circularly polarized left (CL) photons only emphasizes one of the two branches of SS3 and TSS bands, showing clear circular dichroism as reflected in the CR–CL difference spectrum (Fig. 5a and the peak analysis of the MDCs at various energies in Fig. 5c). The obvious dichroic photoemission results are in consistence with the non-degenerate spin configurations in SS3 and TSS, as indicated by the spin-resolved *ab initio* calculations (see Supplementary Fig. 8 in Supplementary Note 6). We note that due to the complexity of the asymmetry of measurement geometry and orbitals effect in CD-ARPES^{36}, we encourage future spin-ARPES measurements for a more quantitative measurement on the spin polarization of TSS and SS3 bands.

## Discussion

Our discovery of the unusual TSSs on these materials establishing them as first examples with non-trivial topological electronic structure showing unusual robustness in Heusler materials with great tenability due to the vast number of compounds in the family. The non-trivial topology in the electronic structure can also help the understanding of various exotic properties recently discovered in half-Heusler compounds, including the large magnetoresistance^{29}, chiral anomaly and Weyl fermions^{37,38} and their unconventional superconductivity^{39,40}. Moreover, the interplay between topological electronic structure and the rich properties in Heusler materials further makes them ideal platforms for the realization of novel topological effects (for example, exotic particles including image monopoles^{41} and axions^{42}) and new topological phases (for example, strain induced topological phase transition^{14} and topological superconductors).

## Methods

## Angle-resolved photoemission spectroscopy

ARPES measurements on single crystals LnPtBi (Ln=Lu, Y) were performed at beamline 10.0.1 of the Advanced Light Source (ALS) at Lawrence Berkeley National Laboratory, USA and beamline I05 of the Diamond Light Source (DLS), UK. The measurement pressure was kept below 3 × 10^{−11}/8 × 10^{−11} Torr in ALS/DLS, and data were recorded by Scienta R4000 analysers at 20 K sample temperature at both facilities. The total convolved energy and angle resolutions were 16 meV/30 meV and 0.2°/0.2° at ALS/DLS, respectively. ARPES circular dichroism measurement was performed at BL5-4 of the Stanford Synchrotron Radiation Lightsource, SLAC national laboratory with 20 eV photons.

*Ab initio* calculations

To simulate a surface, a 54-atomic-layer thick slab model was used with a vacuum more than 10 Å to diminish the coupling between the top and bottom surfaces. The *ab initio* calculations were performed within the framework of the density functional theory and generalized gradient approximation^{43,44}. In the bulk calculations, the density functional theory Bloch wave functions were projected to Wannier functions^{35}, Ln-*d*, Pt-*sd* and Bi-*p* atomic like orbitals. In a half-infinite surface model, we projected the Green function of the bulk to the surface unit cell and obtained the surface local density of states based on the Wannier functions.

We could also calculate the surface bandstructure from tight binding model on the Bi-terminated (111) surface of LuPtBi. The metallic surface states (Fig. 4, SS1–SS3) observed on the Bi-terminated LuPtBi (111) surface all exhibit large spin splitting, thus reflecting very large SOC strength. The surface state SS1 constitutes the FS, in particular, around the and points (Fig. 2). They are mainly composed by Bi-*p*_{z} orbitals of the top Bi layer. The surface Bi atoms form a triangular lattice.

We wrote the effective tight-binding model for the SS1 surface states by considering the nearest neighbour hopping:

(1) About the nearest neighbour hopping. We consider a triangle lattice as illustrated in Supplementary Fig. 9. We take the lattice parameter *a=*1 and in-plane lattice vectors: The six nearest sites of the site 0 are in unit of the lattice vectors: **R**_{1}*=***−R**_{4}*=*(1, 0), **R**_{2}*=***−R**_{5}*=* and **R**_{3}*=***−R**_{6}*=*.

For a single *p*_{z} orbital on the triangular lattice

where *k*_{x}*, k*_{y} are scaled by the unit of .

(2) The Rashba term can be written as

where , and .

The Rashba Hamiltonian is

(3) The Kane–Mele term . In the triangular lattice, the value of depends on the hopping direction, as shown in Supplementary Fig. 9. We derived this term as

We fitted the surface band structure using the parameters *t=*0.35, *α=*0.5 and *β=*0.1 and well reproduced the *ab initio* surface states (Supplementary Figs 9 and 10). Without the Kane–Mele term, the band degeneracy cannot be lifted at the point, although is not time-reversal invariant.

Recently a similar SOC effect^{45} has been employed to describe the surface states on the Tl/Si(111)–(1 × 1) surface^{46}. Existence of strong Rashba effect and the unconventional SOC effect from the surface and the non-centrosymmetric bulk induces significant effect such as weak antilocalization and high mobility in transport measurements, and makes the LnPtBi a feasible candidate for spintronics applications.

## Data availability

All relevant data are available on request, which should be addressed to Y.L.C.

## Additional information

**How to cite this article:** Liu, Z. K. *et al.* Observation of unusual topological surface states in half-Heusler compounds LnPtBi (Ln=Lu, Y). *Nat. Commun.* **7,** 12924 doi: 10.1038/ncomms12924 (2016).

## References

- 1.
Qi, X. & Zhang, S.-C. Topological insulators and superconductors.

*Rev. Mod. Phys.***83**, 1057–1110 (2011). - 2.
Hasan, M. Z. & Kane, C. L. Colloquium: topological insulators.

*Rev. Mod. Phys.***82**, 3045 (2010). - 3.
Ando, Y. Topological insulator materials.

*J. Phys. Soc. Jpn***82**, 102001 (2013). - 4.
Yan, B. & Zhang, S.-C. Topological materials.

*Rep. Prog. Phys.***75**, 096501 (2012). - 5.
Hsieh, T. H.

*et al.*Topological crystalline insulators in the SnTe material class.*Nat. Commun.***3**, 982 (2012). - 6.
Dziawa, P.

*et al.*Topological crystalline insulator states in Pb_{1−x}Sn_{x}Se.*Nat. Mater.***11**, 1023–1027 (2012). - 7.
Liu, Z. K.

*et al.*Discovery of a three-dimensional topological dirac semimetal, Na_{3}Bi.*Science***343**, 864–867 (2014). - 8.
Liu, Z. K.

*et al.*A stable three-dimensional topological dirac semimetal Cd_{3}As_{2}.*Nat. Mater.***13**, 677–681 (2014). - 9.
Xu, S.-Y.

*et al.*Discovery of a Weyl fermion semimetal and topological Fermi arcs.*Science***349**, 613–617 (2015). - 10.
Lv, B. Q.

*et al.*Experimental discovery of Weyl semimetal TaAs.*Phys. Rev. X***5**, 031013 (2015). - 11.
Yang, L. X.

*et al.*Weyl semimetal phase in the non-centrosymmetric compound TaAs.*Nat. Phys.***11**, 728–732 (2015). - 12.
Chadov, S.

*et al.*Tunable multifunctional topological insulators in ternary Heusler compounds.*Nat. Mater.***9**, 541–545 (2010). - 13.
Lin, H.

*et al.*Half-Heusler ternary compounds as new multifunctional experimental platforms for topological quantum phenomena.*Nat. Mater.***9**, 546–549 (2010). - 14.
Ruan, J.

*et al.*Symmetry-protected ideal Weyl semimetal in HgTe-class materials.*Nat. Commun.***7**, 11136 (2016). - 15.
Canfield, P. C.

*et al.*Magnetism and heavy fermion-like behavior in the RBiPt series.*J. Appl. Phys.***70**, 5800 (1991). - 16.
Aoki, Y., Sato, H. R., Sugawara, H. & Sato, H. Anomalous magnetic properties of Heusler superconductor YbPd

_{2}Sn.*Phys. C: Supercond.***333**, 187–194 (2000). - 17.
Butch, N. P., Syers, P., Kirshenbaum, K., Hope, A. P. & Paglione, J. Superconductivity in the topological semimetal YPtBi.

*Phys. Rev. B***84**, 220504 (2011). - 18.
Goll, G.

*et al.*Thermodynamic and transport properties of the non-centrosymmetric superconductor LaBiPt.*Phys. B: Condens. Matter***403**, 1065–1067 (2008). - 19.
Tafti, F. F.

*et al.*Superconductivity in the noncentrosymmetric half-Heusler compound LuPtBi: a candidate for topological superconductivity.*Phys. Rev. B***87**, 184504 (2013). - 20.
Fisk, Z.

*et al.*Massive electron state in YbBiPt.*Phys. Rev. Lett.***67**, 3310 (1991). - 21.
Xu, G.

*et al.*Weak antilocalization effect and noncentrosymmetric superconductivity in a topologically nontrivial semimetal LuPdBi.*Sci. Rep.***4**, 5709 (2014). - 22.
Pan, Y.

*et al.*Superconductivity and magnetic order in the noncentrosymmetric half-Heusler compound ErPdBi.*Europhys. Lett.***104**, 27001 (2013). - 23.
Yan, B. & de Visser, A. Half-Heusler topological insulator.

*MRS Bull.***39**, 859–866 (2014). - 24.
Feng, W., Wen, J., Zhou, J., Xiao, D. & Yao, Y. First-principles calculation of topological invariants within the FP-LAPW formalism.

*Comput. Phys. Commun.***183**, 1849–1859 (2012). - 25.
Fu, L. & Berg, E. Odd-parity topological superconductors: theory and application to Cu

_{x}Bi_{2}Se_{3}.*Phys. Rev. Lett.***105**, 097001 (2010). - 26.
Xiao, D.

*et al.*Half-Heusler compounds as a new class of three-dimensional topological insulators.*Phys. Rev. Lett.***105**, 096404 (2010). - 27.
Liu, C.

*et al.*Metallic surface electronic state in half-Heusler compounds RPtBi (R=Lu, Dy, Gd).*Phys. Rev. B***83**, 205133 (2011). - 28.
Chandra, S.

*et al.*Large linear magnetoresistance and weak anti-localization in Y(Lu)PtBi topological insulators. Preprint at http://arxiv.org/abs/arXiv:1502.00604 (2015). - 29.
Hou, Z.

*et al.*Extremely high electron mobility and large magnetoresistance in the half-Heusler semimetal LuPtBi.*Phys. Rev. B***92**, 235134 (2015). - 30.
Chen, Y. L. Studies on the electronic structures of three-dimensional topological insulators by angle resolved photoemission spectroscopy.

*Front. Phys.***7**, 175–192 (2012). - 31.
Chu, R.-L., Shan, W.-Y., Lu, J. & Shen, S.-Q. Surface and edge states in topological semimetals.

*Phys. Rev. B***83**, 075110 (2011). - 32.
Wu, S.-C., Yan, B. H. & Felser, C. Ab initio study of topological surface states of strained HgTe.

*Europhys. Lett.***107**, 57006 (2014). - 33.
Brüne, C.

*et al.*Quantum Hall effect from the topological surface states of strained bulk HgTe.*Phys. Rev. Lett.***106**, 126803 (2011). - 34.
Sancho, M. P. L., Sancho, J. M. L. & Rubio, J. Quick iterative scheme for the calculation of transfer matrices: application to Mo (100).

*J. Phys. F: Metal Phys.***14**, 1205 (1984). - 35.
Mostofi, A. A.

*et al.*wannier90: A tool for obtaining maximally-localised Wannier functions.*Comput. Phys. Commun.***178**, 685–699 (2008). - 36.
Schönhense, G., Westphal, C., Bansmann, J. & Getzlaff, M. Circular dichroism in photoemission from nonmagnetic, low-Z solids: a conspicuous effect of the photon spin.

*Europhys. Lett.***17**, 727 (1992). - 37.
Hirschberger, M.

*et al.*The chiral anomaly and thermopower of Weyl fermions in the half-Heusler GdPtBi. Preprint at http://arxiv.org/abs/arXiv:1602.07219 (2016). - 38.
Shekhar, C.

*et al.*Observation of chiral magneto-transport in RPtBi topological Heusler compounds. Preprint at http://arxiv.org/abs/arXiv:1604.01641v1 (2016). - 39.
Kim, H.

*et al.*Beyond spin-triplet: nodal topological superconductivity in a noncentrosymmetric semimetal. Preprint at http://arxiv.org/abs/arXiv:1603.03375v2 (2016). - 40.
Nakajima, Y.

*et al.*Topological RPdBi half-Heusler semimetals: a new family of noncentrosymmetric magnetic superconductors.*Sci. Adv.***1**, 5 (2015). - 41.
Qi, X.-L., Li, R., Zang, J. & Zhang, S.-C. Inducing a magnetic monopole with topological surface states.

*Science***323**, 1184–1187 (2009). - 42.
Li, R., Wang, J., Qi, X.-L. & Zhang, S.-C. Dynamical axion field in topological magnetic insulators.

*Nat. Phys.***6**, 284–288 (2010). - 43.
Kresse, G. & Hafner, J. Ab initio molecular dynamics for liquid metals.

*Phys. Rev. B***47**, 558–561 (1993). - 44.
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple.

*Phys. Rev. Lett.***77**, 3865–3868 (1996). - 45.
Nakajin, K. & Murakami, S. Theory of unconventional spin states in surfaces with non-Rashba spin–orbit interaction.

*Phys. Rev. B***91**, 245428 (2015). - 46.
Sakamoto, K.

*et al.*Abrupt rotation of the Rashba spin to the direction perpendicular to the surface.*Phys. Rev. Lett.***102**, 096805 (2009).

## Acknowledgements

Y.L.C. acknowledges the support of the EPSRC Platform Grant (Grant No. EP/M020517/1) and Hefei Science Center CAS (2015HSC-UE013). C.F. acknowledges the financial support by the ERC Advanced Grant (No. 291472 ‘Idea Heusler’). J.J. acknowledges the support of the NRF, Korea through the SRC Center for Topological Matter (No. 2011-0030787). The ALS is supported by the Office of Basic Energy Sciences of the U.S. DOE under Contract No. DE-AC02-05CH11231. H.F.Y. acknowledges the finacial support from the Bureau of Frontier Sciences and Education, Chinese Academy of Sciences.

## Author information

## Affiliations

### School of Physical Science and Technology, ShanghaiTech University and CAS-Shanghai Science Research Center, Shanghai 201203, China

- Z. K. Liu
- , J. Jiang
- , B. Yan
- & Y. L. Chen

### State Key Laboratory of Low Dimensional Quantum Physics, Department of Physics and Collaborative Innovation Center for Quantum Matter, Tsinghua University, Beijing 100084, China

- L. X. Yang
- & Y. L. Chen

### Max Planck Institute for Chemical Physics of Solids, D-01187 Dresden, Germany

- S.-C. Wu
- , C. Shekhar
- , B. Yan
- & C. Felser

### Advanced Light Source, Lawrence Berkeley National Laboratory, Berkeley, California 94720, USA

- J. Jiang
- , Y. Zhang
- , S.-K. Mo
- & Z. Hussain

### State Key Laboratory of Functional Materials for Informatics, SIMIT, Chinese Academy of Sciences, Shanghai 200050, China

- H. F. Yang

### Physics Department, Oxford University, Oxford OX1 3PU, UK

- Y. L. Chen

## Authors

### Search for Z. K. Liu in:

### Search for L. X. Yang in:

### Search for S.-C. Wu in:

### Search for C. Shekhar in:

### Search for J. Jiang in:

### Search for H. F. Yang in:

### Search for Y. Zhang in:

### Search for S.-K. Mo in:

### Search for Z. Hussain in:

### Search for B. Yan in:

### Search for C. Felser in:

### Search for Y. L. Chen in:

## Contributions

Y.L.C. conceived the experiments. Z.K.L. and L.X.Y. carried out ARPES measurements with the assistance of J.J., H.F.Y., Y.Z. and S.-K.M. C.S. synthesized and characterized the bulk single crystals. S.-C.W. and B.Y. performed *ab initio* calculations. All authors contributed to the scientific planning and discussions.

## Competing interests

The authors declare no competing financial interests.

## Corresponding author

Correspondence to Y. L. Chen.

## Supplementary information

## PDF files

- 1.
### Supplementary Information

Supplementary Figures 1-10 and Supplementary Notes 1-6

- 2.
### Peer Review File

## Comments

By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.

This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/